Analysis of high loss viscoelastic composites


 Kory Fleming
 1 years ago
 Views:
Transcription
1 Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science Program and Rheology Research Center University of WisconsinMadison 47 Engineering Research Building 500 Engineering Drive, Madison, WI adapted from J. Materials Science, 28, , (993). Address correspondence to R. Lakes Synopsis A theoretical study of viscoelastic properties of composites is presented with the aim of identifying structures which give rise to a combination of high stiffness and high loss tangent. Laminates with Voigt and Reuss structure, as well as composite materials attaining the HashinShtrikman bounds on stiffness were evaluated via the correspondence principle. Similarly, viscoelastic properties of composites containing spherical or platelet inclusions were explored. Reuss laminates and platelet filled materials composed of a stiff, low loss phase and a compliant high loss phase were found to exhibit high stiffness combined with high loss tangent. INTRODUCTION Viscoelastic materials can be of use in the damping of mechanical vibration and in the absorption of sound. The loss tangent, or tangent of the phase angle δ between stress and strain in sinusoidal loading, is a useful measure of material damping. Most materials used in structural applications, however, have small loss tangents. Conversely, materials with high loss tangents tend to be compliant, hence not of structural interest. Fig. contains a stiffnessloss map (plot of the absolute value of the dynamic modulus vs loss tangent) for some representative materials. Compliant, lossy materials are used as layers over stiff materials in various applications; nevertheless a stiff material with high loss would be of use in structural damping of noise and vibration. We consider in this article the possibility of making composite microstructures providing high stiffness and high loss. A possible avenue for making high loss composites is to make use of nonaffine deformation. This is in contrast to affine deformation in which the particles in the solid move in a way corresponding to a uniform strain plus a rotation in a continuum. The negative Poisson's ratio materials developed by Lakes (987) exhibit this property in that the foam cells unfold during deformation (Lakes, 99; Chen and Lakes, 99). Non
2 affine deformation can result in high viscoelastic loss in a composite if the phase which has the highest loss experiences a larger strain than does the composite as a whole. Elastic properties of multiphase composite materials have been studied extensively. Of these studies, the ones most relevant to the present work are those dealing with bounds on the elastic behavior and predicted properties of composites of relatively simple structure. The upper and lower bounds of stiffness of two phase and many phase composite materials have been obtained in terms of volume fraction of constituents (Hashin, 962; Hashin and Shtrikman, 963). Bounds and expressions for the effective elastic moduli of materials reinforced by parallel hollow circular fibers in hexagonal or random arrays have also been derived by a variational method (Hashin, 962). Furthermore, bounds on three independent effective elastic moduli of an nphase fiber reinforced composite of arbitrary transverse phase geometry, plane strain bulk modulus, transverse shear modulus and shear modulus in plane parallel to fibers, have been derived in terms of phase volume fractions(hashin, 965a). For viscoelastic heterogeneous media of several discrete linear viscoelastic phases with known stressstrain relations, it was shown that the effective relaxation and creep functions could be obtained by the correspondence principle of the theory of linear viscoelasticity (Hashin, 965b). In some cases explicit results in terms of general linear viscoelastic matrix properties was given, and thus permitting direct use of experimental information (Hashin, 966). In a review by Ahmed and Jones (990) of particulate reinforcement theories for polymer composites, it was concluded that the macroscopic behavior was affected by the size, shape, distribution, and interfacial adhesion of the inclusions. This article makes use of some of these results for elastic composites to explore accessible regions of the stiffnessloss maps of the materials. ELASTIC AND VISCOELASTIC PROPERTIES OF COMPOSITES For the simplest case of a twophase composite, the Voigt and Reuss composites described below represent rigorous upper and lower bounds on the Young's modulus for a given volume fraction of one phase. The HashinShtrikman composites represent upper and lower bounds for isotropic elastic composites. Viscoelastic composites containing spherical or platelet inclusions are also considered. Results obtained via the correspondence principle are plotted as "stiffnessloss maps" in the subsequent section. Voigt composite Let phase be stiff; let phase 2 be high loss. The geometry of the Voigt model structure is shown in Figure 2. The composite can contain laminations as shown in Figure (a) or it can be made of continuous fibers in Figure (b); in either case the strain in each phase is the same. For an elastic material with one of these structures, the Voigt relation is E c = E V + E 2 V 2, in which E c, E and E 2 refer to the Young's modulus of the composite, phase and phase 2, and V and V 2 refer to the volume fraction of phase and phase 2 with V +V 2 =. The Voigt relation for the stiffness of an elastic composite is obtained by recognizing that for the given geometry, the strain in each phase is the same; the forces in each phase are additive. By the correspondence principle (Hashin, 970, Christensen, 980), the elastic relation can be converted to a steady state harmonic viscoelastic relation by replacing the Young's moduli E by E * (iω) or E *, in which ω is the angular frequency of the harmonic loading. This procedure gives E c * = E * V + E 2 * V2 ()
3 with E * = E' + i E" and loss tangent tan δ = E"/E'. Taking the ratio of real and imaginary parts, we obtain the loss tangent of the composite tan δ c = E c "/E c '. V tanδ + V E 2 ' 2 tanδ 2 tan δ c = E ' V + E 2 ' E ' V 2 Reuss composite The geometry of the Reuss model structure is shown in Figure (c); each phase experiences the same stress. For elastic materials, /E c = V /E + V 2 /E 2. Again using the correspondence principle, the viscoelastic relation is obtained as E c * = V E * + V 2 E 2 * (3) Again separating the real and imaginary parts of E c *, the loss tangent of the composite tan δ c is obtained: E (tanδ +tanδ 2 )[V +V ' 2 E tan δ c = 2 ' ](tanδ tanδ 2 )[V tanδ 2 +V 2 tanδ E ' E 2 ' ] E (tanδ tanδ 2 )[V +V ' 2 E 2 ' ]+(tanδ +tanδ 2 )[V tanδ 2 +V 2 tanδ E ' (4) E 2 ' ] (2) HashinShtrikman composite: arbitrary twophase geometry Allowing for 'arbitrary' phase geometry, the upper and lower bounds on the elastic moduli as a function of composition have been developed using variational principles. The lower bound for the shear modulus G L of the composite was given as (Hashin and Shtrikman, 963) V G L = G 2 + G G + 6(K 2 +2G 2 )V (5) 2 2 5(3K 2 +4G 2 )G 2 in which K, G and V, and G 2 and V 2 are the bulk modulus, shear modulus and volume fraction of phases, and 2, respectively. Here G >G 2, so that G L represents the lower bound on the shear modulus. Interchanging the numbers and 2 in Equation(5) results in the upper bound G U for the shear modulus. As for viscoelastic materials, we again apply the correspondence principle. The complex viscoelastic shear moduli of the composite G L * and G U * are obtained as G L * = G2 * V + G * G2 * + 6(K 2 * +2G2 * )V2 5(3K 2 * +4G2 * )G2 * and (6)
4 G U * = G * V + 2 G 2 * G * + 6(K * +2G * (7) )V 5(3K * +4G * )G * In these cases the loss tangent is more complicated to write explicitly, so it is more expedient to graphically display computed numerical values. Hashin transversely isotropic fiber reinforced composites This case is of interest since it allows more than two phases, a situation applicable to the analysis of experimental results in a companion article. For two phases the results are almost identical to the arbitrary phase geometry case considered above. The shear modulus of elastic multiphase transversely isotropic fiber reinforced composites of arbitrary transverse phase geometry, can be bounded from below and above in terms of phase moduli and phase volume fractions. The lower and upper bounds on the shear modulus m ( ) and m (+) were given for elastic composites (Hashin, 965a) as and m () = G + 2G (K +G ) K +2G r=n {[ r=2 (G r G )V r G +K G /(K +2G )]  }  (8) m (+) = G n + 2G n (K n +G n ) K n +2G n {[ r=n (G r G n )V r G r +K n G n /(K n +2G n )]  }  (9) r= in which n is the number of the phases, G and K are the shear and bulk moduli of the most compliant phase, G n and K n are the shear and bulk moduli of the stiffest phase. r is a free index representing the phase number; phases are numbered in order of increasing stiffness. On the basis of the correspondence principle, corresponding results for the complex shear modulus (not necessarily bounds) of the composites are again obtained by replacing m(), m(+), G, K, G r and G n by G L *, GU *, G *, K *, Gr * and G n * in Equations(8) and (9), respectively. The loss tangent again is complicated to write explicitly, so it is graphically displayed using computed numerical values. Spherical particulate inclusions For a small volume fraction V =  V 2 of spherical elastic inclusions in a continuous phase of another elastic material, the shear modulus of the composite G c was given as(christensen, 979) G c G =  5(ν ) (  G 2 G )V 2 75ν +2(45ν ) G 2 G (0) in which ν is the Poisson's ratio of phase, and phase and phase 2 represent the matrix material and the inclusion material respectively. Using the correspondence principle again and assuming there is no relaxation in Poisson's ratio, Equation(0) becomes
5 G c * = G * 5(ν  ) (G *  G 2 * )V 2 75ν +2(45ν ) G 2 * () G * for the complex shear modulus of the composite material. The loss tangent again is complicated to write explicitly, so it is graphically displayed using computed numerical values. Platelet inclusions For a dilute suspension of platelet elastic inclusions of phase 2 in a matrix of phase, the shear modulus of the composite G c was given as(christensen, 979) G c = G + V 2 (G 2 G ) 5 [ 9K 2 +4(G +2G 2 ) K G 3 G G 2 ] (2) 2 Again, using the correspondence principle, Equation(2) becomes G c * = G * + V 2 (G 2 * G * ) 5 [ 9K 2 * +4(G * +2G2 * ) G K 2 * G 2 * + 6 * G 2 *] (3) for the complex shear modulus of the composite materials. As for procedure, we remark that although Equations (5) to (3) were developed for the shear modulus of the composite, the shear moduli G * were replaced by the Young's moduli E * in the figures for comparison with Fig.. The Voigt and Reuss relations given by Equations () and (3) apply to G * as well as to E *. The actual relationship between E * and G * and the properties of the constituents of a composite is simple only for certain phase geometries. For example, for some common phase geometries, a Poisson's ratio of 0.3 for each phase gives a Poisson's ratio close to or equal to 0.3 for the composite. However for some phase geometries, a constituent Poisson's ratio of 0.3 can give rise to a negative Poisson's ratio in cellular solids with one phase void (Lakes, 987) or in unusual laminates (Milton, in press). The calculations are on the basis that V +V 2 = except that V +V 2 =0.8 for the multiphase Hashin elastic bound, for which 20% void by volume fraction is assumed to be contained as a third phase in the composite. RESULTS AND DISCUSSION Results are plotted as stiffnessloss maps (plots of E * vs tan δ) as shown in Figures 24 below. Figure 2 shows predicted properties of composites containing phases which differ greatly in properties. Steel is considered as phase, with E * =200 GPa, tan δ = 0.00 and and a viscoelastic elastomer as phase 2, with E 2 * =0.020 GPa, tan δ2 =.0. The graph was enlarged in the vicinity of 00% phase and shown in Figure 3 for clarity. A small volume fraction of phase 2 results in a large increase in loss with little reduction in stiffness so that the Reuss structure permits higher losses than the Voigt structure. However, in the Reuss structure each phase carries the full stress, so that a composite of this type will not be strong if, as is usual, the soft phase 2 is weak. As for 'bounds' on the properties, the curves for the Voigt and Reuss composites enclose a region in the stiffnessloss map, as do the curves for the upper and lower Hashin Shtrikman composites. It is tempting to think of these curves as 'bounds' on the viscoelastic behavior, however such a surmise has not been proven. They represent extremes of composites which can be fabricated, however we do not yet know if they
6 represent true bounds. Roscoe (969) has mathematically established bounds for the real and imaginary parts E ' and E '' of the complex modulus of composites and has shown them to be equivalent to the Voigt and Reuss relations. Therefore the stiffness, expressed as E * of the composite is bounded from above by the Voigt limit and cannot exceed the stiffness of the stiff phase. This is not quite the same as establishing bounds for a stiffnessloss map since it is not obvious whether a maximum in tan δ = E"/E' could be obtained simultaneously with a maximum in E'. In particular, we can construct tan δ c = E" voigt /E' reuss > E" reuss /E' reuss and be within the bounds of Roscoe. We do not yet know if such a composite is physically realizable. In the stiffnessloss map, the lower and upper twophase Hashin composites behave similarly to the Voigt and Reuss composites, respectively. This is in contrast to the usual plots of elastic stiffness vs volume fraction, in which the Hashin bounds can differ greatly from the Voigt/Reuss ones. As for the physical attainment of the Voigt and Reuss composites, simple laminates can be made as in Fig., but these are anisotropic. Isotropic composites which attain the Voigt or Reuss moduli are not considered to be attainable. Isotropic polycrystals attaining the Voigt or Reuss bounds for the bulk modulus are also possible (Avellaneda and Milton, 989) at the expense of some added structural complexity. For the threephase Hashin structure with 20% void content in the composite, the lower curve reduces to zero and is not shown in the graph; the upper bound lies close to the Voigt curve with 20% to 40% lower stiffness as shown in Fig. 2. The composite containing soft spherical inclusions is also found to behave similarly to the Voigt composite in that a small volume fraction of soft, viscoelastic material has a minimal effect on the loss tangent, though it does reduce the stiffness. As for the composite containing soft platelet inclusions, it is found that the results are similar to those of the Reuss structure. A small volume fraction of platelet inclusions as phase 2 results in a very large increase in loss tangent without any significant reduction in the stiffness. However, soft platelets resemble pennyshaped cracks in the matrix, so that such a composite would be weaker than the matrix, particularly if the matrix were brittle. Figure 4 shows predicted properties of composites containing phases which do not differ so much in properties as steel and viscoelastic elastomers. Copper as phase, with E * =7 GPa, tanδ = and indium as phase 2, with E 2 * =0.8 GPa, tanδ2 =0.025 (at khz) were used for this investigation. Observe that the shape of this stiffnessloss map differs from the case of the polymermetal composite. The implication of this difference in shape is as follows. If the constituents differ by orders of magnitude in stiffness and loss, then the Reuss and platelet composites are orders of magnitude superior to the Voigt and spherical inclusion composites in achieving high stiffness and high loss. If the constituents do not differ so much in their properties, their composites of various structures do not differ as much either. Composites containing a stiff, low loss material (such as a metal) and a small amount of compliant, high loss material can exhibit a stiffness close to that of the metal, as well as high loss superior to that of a metalmetal composite. An interesting aspect of the Reuss and platelet composites which give the highest loss (for given stiffness) is that they exhibit highly nonuniform strain fields. The strain in the soft, lossy phase is much larger than the strain in the stiff phase. This is in contrast to the Voigt composite in which the strain in each phase is the same. The reentrant foams (Chen and Lakes, 989, in press) with a negative Poisson's ratio also exhibit nonaffine deformation of a more complex nature in that the foam cells unfold as the foam is deformed. CONCLUSIONS
7 . In a stiffnessloss map, the upper and lower twophase Hashin composites behave similarly to the Voigt and Reuss composites, respectively. 2. Reuss laminates and platelet filled materials based on a stiff, low loss phase and a compliant high loss phase were found to exhibit high stiffness combined with high loss tangent. However, in the Reuss structure each phase carries the full stress, so that a composite of this type will not be strong if, as is usual, the compliant phase is weak. 3. A composite containing soft lossy spherical inclusions in a stiff matrix behaves similarly to the Voigt composite: low loss and a reduction in stiffness. 4. Composites containing a metal and a small amount of compliant, high loss polymer can in principle exhibit a stiffness close to that of the metal, as well as high loss. ACKNOWLEDGMENT We thank the ONR for their support of this work. We also thank the University of Iowa for a University Faculty Scholar Award to one of the authors (RSL). REFERENCES Ahmed, S., and Jones, F.R. (990), "A review of particulate reinforcement theories for polymer composites", J. Materials Sci., 25, Avellaneda, M. and Milton, G., (989) "Optimal bounds on the effective bulk modulus of polycrystals", SIAM J. Appl. Math. 49, Chen, C.P. and Lakes, R.S., (99) "Holographic study of conventional and negative Poisson's ratio metallic foams: elasticity, yield, and microdeformation", J. Materials Science 26, Chen, C.P. and Lakes, R.S., (989)"Dynamic wave dispersion and loss properties of conventional and negative Poisson's ratio polymeric cellular materials", Cellular polymers, 8, Christensen, R.M., Theory of viscoelasticity, 2nd ed., Academic Press, New York, 982. Christensen, R.M., Mechanics of composite materials, John Wiley & Sons, New York, 979. Ferry, J. D. Viscoelastic properties of Polymers, 2nd ed J. Wiley, N.Y., 979 Hashin, Z., (962) "The elastic moduli of heterogeneous materials", J. Appl. Mech., Trans. ASME, 84E, Hashin Z., and B. W. Rosen, (964),"The elastic moduli of fiberreinforced materials", J. Appl. Mech., Trans. ASME, 3, Hashin, Z., (965a),"On elastic behaviour of fibre reinforced materials of arbitrary transverse phase geometry", J. Mech. Phys. solids, 3, Hashin, Z., (965b), "Viscoelastic behavior of heterogeneous media", J. Appl. Mech., Trans. ASME, 32E,
8 Hashin, Z., (966), "Viscoelastic fiber reinforced materials", AIAA Jnl., 4, Hashin, Z., (970), "Complex moduli of viscoelastic composites: I. General theory and application to participate composites", Int. J. Solids, Structures, 6, Hashin Z., and Shtrikman, S. (963),"A variational approach to the theory of the elastic behavior of multiphase materials", J. Mech. Phys. solids,, Katz, J. L. (97),"Hard tissue as a composite material  I. Bounds on the elastic behavior", J. Biomechanics, 4, Lakes, R.S. (987),"Foam structures with a negative Poisson's ratio", Science, 235, Lakes, R.S. (99), "Deformation mechanisms of negative Poisson's ratio materials: structural aspects", J. Materials Science, 26, Lakes, R.S., Katz, J.L., and Sternstein, S.S., (979), "Viscoelastic properties of wet cortical bone: Part I, torsional and biaxial studies." Journal of Biomechanics, 2, Milton, G., (in press) "Laminates with a negative Poisson's ratio". Nielsen, I., Mechanical Properties of Polymers, Reinhold, 962. Nowick A. S. and Berry, B. S.Anelastic relaxation in crystalline solids, Academic, N.Y., 972. Roscoe, R., (969), "Bounds for the real and imaginary parts of the dynamic moduli of composite viscoelastic systems", J. Mech. Phys. Solids, 7, Shipkowitz, A.T., Chen, C.P. and Lakes, R.S., (988), "Characterization of highloss viscoelastic elastomers", Journal of Materials Science, 23, Zener, C. Elasticity and anelasticity of metals, University of Chicago Press, 948.
9 Figures 000 E(GPa) Steel Copper Aluminum Bone Polystyrene PMMA Polycarbonate.0 Hevea rubber High loss elastomer tan δ. Stiffness vs loss tangent for some representative materials at or near room temperature. Steel, Hz, after Nowick and Berry (972) Copper, 600 Hz, after Nowick and Berry (972) Polymethyl methacrylate, (PMMA), 0 Hz and khz, after Ferry (979) Bone, 00 Hz, after Lakes, Katz, Sternstein (979) Hevea rubber, 0 Hz2 khz, after Ferry (979) Polystyrene, 00 Hz, khz, after Ferry (979) Polycarbonate, 00 Hz, after Nielsen (962) Viscoelastic elastomer, 00,,000 Hz, after Shipkowitz, et. al. (988) (a) (b) (c) 2. (a) Laminated Voigt structure. (b) Fibrous Voigt structure. (c) Reuss structure.
10 0 3 Platelet Vi: % Phase Reuss V: % Platelet Vi: 0.00% 0 2 Spherical VI: 0% Hashin V: 99.9% E* ( GPa ) Voigt V: 0% Hashin, 3 phase V: 5% V2: 65% 03 Voigt V: % Hashin V: 0% 02 Spherical Vi: 45% Hashin, 3 phase V: % V2: 79% tanδ Reuss V: 99% Reuss V: 50% Phase Stiffnessloss map for composites of steel as phase and viscoelastic elastomer as phase 2. x: Voigt curve, +: Reuss curve, : twophase Hashin curve, : upper curve of threephase Hashin composite with 20% voids as one phase. o: composite with phase 2 as dilute spherical inclusions. _ : composite with phase 2 as dilute platelet inclusions.
11 0 3 Reuss V2: 0.000% E* ( GPa ) Phase Platelet Vi: 0.000% Platelet Vi: % Spherical Vi: 5% Spherical Vi: 25% Voigt V2: 25% tan δ Stiffnessloss map for composites of steel as phase and viscoelastic elastomer as phase 2; expanded plot of upper left portion of Fig. 3. x: Voigt curve, +: Reuss curve, : upper curve of threephase Hashin composite with 20% voids as one phase. o: composite with phase 2 as dilute spherical inclusions. _ : composite with phase 2 as dilute platelet inclusions.
12 0 3 Platelet Vi: 0.5% Spherical Vi: 0% Reuss V: 99% Hashin V: 97% Platelet Vi: 3% Spherical Vi: 30% E* ( GPa ) Phase 03 Voigt V: 75% Hashin, 3 phase V: 60% V2: 20% Hashin V: 50% Voigt V: 25% 02 tanδ Reuss V: 75% Phase 2 Hashin, 3 phase V: 30% V2: 50% 05. Stiffnessloss map for composites of copper as phase and indium as phase 2. x: Voigt bound, +: Reuss curve, : twophase Hashin curve, : upper curve of threephase Hashin composite with 20% voids as one phase. o: composite with phase 2 as dilute spherical inclusions. _ : composite with phase 2 as dilute platelet inclusions.
Module 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationCellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).
1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, 475477 (1996). Abstract Material microstructures are presented which can exhibit coefficients
More informationH Kalathur 1, 2 1, 2,3. , R S Lakes. 3
Column dampers with negative stiffness: high damping at small amplitude adapted from Kalathur, H., Lakes, R. S., Column dampers with negative stiffness: high damping at small amplitude, Smart Materials
More informationDesign of a fastener based on negative Poisson's ratio foam adapted from
1 Design of a fastener based on negative Poisson's ratio foam adapted from Choi, J. B. and Lakes, R. S., "Design of a fastener based on negative Poisson's ratio foam", Cellular Polymers, 10, 205212 (1991).
More informationMSE 383, Unit 33. Joshua U. Otaigbe Iowa State University Materials Science & Engineering Dept.
Dynamic Mechanical Behavior MSE 383, Unit 33 Joshua U. Otaigbe Iowa State University Materials Science & Engineering Dept. Scope Why DMA & TTS? DMA Dynamic Mechanical Behavior (DMA) Superposition Principles
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationDynamic Mechanical Analysis (DMA) of Polymers by Oscillatory Indentation
Dynamic Mechanical Analysis (DMA) of Polymers by Oscillatory Indentation By Jennifer Hay, Nanomechanics, Inc. Abstract This application note teaches the theory and practice of measuring the complex modulus
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationFinite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure
Vibrations in Physical Systems Vol.26 (2014) Finite Element Analysis of Dynamic Properties of Thermally Optimal Twophase Composite Structure Abstract Maria NIENARTOWICZ Institute of Applied Mechanics,
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationFrancisco Paulo Lépore Neto. Marcelo Braga dos Santos. Introduction 1. Nomenclature. Experimental Apparatus and Formulation
Francisco Paulo Lépore Neto and Marcelo Braga dos Santos Francisco Paulo Lépore Neto fplepore@mecanica.ufu.br Federal University of Uberlandia School of Mechanical Engineering 38408902 Uberlandia, MG,
More informationProperties of a chiral honeycomb with a Poisson's ratio 1
Properties of a chiral honeycomb with a Poisson's ratio 1 D. Prall, R. S. Lakes Int. J. of Mechanical Sciences, 39, 305314, (1996). Abstract A theoretical and experimental investigation is conducted
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationThe Influence of Strain Amplitude, Temperature and Frequency on Complex Shear Moduli of Polymer Materials under Kinematic Harmonic Loading
Mechanics and Mechanical Engineering Vol. 21, No. 1 (2017) 157 170 c Lodz University of Technology The Influence of Strain Amplitude, Temperature and Frequency on Complex Shear Moduli of Polymer Materials
More informationD Y N A M I C M E C H A N I C A L A N A L Y S I S A N D I T S A D V A N T A G E S O V E R D E F L E C T I O N T E M P E R A T U R E U N D E R L O A D
D Y N A M I C M E C H A N I C A L A N A L Y S I S A N D I T S A D V A N T A G E S O V E R D E F L E C T I O N T E M P E R A T U R E U N D E R L O A D Sujan E. Bin Wadud TA Instruments 9 Lukens Drive, New
More informationUSING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE
Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and
More informationNegative incremental bulk modulus in foams
Philosophical Magazine Letters, Vol. 86, No., October 6, 65 659 Negative incremental bulk modulus in foams B. MOOREy, T. JAGLINSKIz, D. S. STONEyz and R. S. LAKES*zx{ ydepartment of Materials Science and
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationSession 11: Complex Modulus of Viscoelastic Polymers
Session 11: Complex Modulus of Viscoelastic Polymers Jennifer Hay Factory Application Engineer NanoScale Sciences Division Agilent Technologies jenny.hay@agilent.com To view previous sessions: https://agilenteseminar.webex.com/agilenteseminar/onstage/g.php?p=117&t=m
More informationEffects of geometry and properties of fibre and matrix on overall. composite parameters
Int. Journal of Applied Sciences and ngineering Research, ol. 3, Issue 4, 2014 www.ijaser.com 2014 by the authors Licensee IJASR Under Creative Commons License 3.0 editorial@ijaser.com Research article
More informationComputational studies on highstiffness, highdamping SiC InSn particulate reinforced composites
International Journal of Solids and Structures 39 (2002) 5799 5812 www.elsevier.com/locate/ijsolstr Computational studies on highstiffness, highdamping SiC InSn particulate reinforced composites Hyung
More informationSound Propagation through Media. Nachiketa Tiwari Indian Institute of Technology Kanpur
Sound Propagation through Media Nachiketa Tiwari Indian Institute of Technology Kanpur LECTURE13 WAVE PROPAGATION IN SOLIDS Longitudinal Vibrations In Thin Plates Unlike 3D solids, thin plates have surfaces
More information2.1 Strain energy functions for incompressible materials
Chapter 2 Strain energy functions The aims of constitutive theories are to develop mathematical models for representing the real behavior of matter, to determine the material response and in general, to
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationA multiscale approach for composite materials as multifield continua
Materials Science Forum Vols. 539543 (27) pp. 25512556 online at http://www.scientific.net (27) Trans Tech Publications, Switzerland A multiscale approach for composite materials as multifield continua
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationStatistical continuum mechanics analysis of an elastic twoisotropicphase composite material
Composites: Part B 31 (2000) 39 46 www.elsevier.com/locate/compositesb Statistical continuum mechanics analysis of an elastic twoisotropicphase composite material S. Lin, H. Garmestani* Mechanical Engineering
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationEffect of Strain Hardening on Unloading of a Deformable Sphere Loaded against a Rigid Flat A Finite Element Study
Effect of Strain Hardening on Unloading of a Deformable Sphere Loaded against a Rigid Flat A Finite Element Study Biplab Chatterjee, Prasanta Sahoo 1 Department of Mechanical Engineering, Jadavpur University
More informationMechanical characterization of visco termo elastic properties of a polymer interlayer by dynamic tests
Mechanical characterization of visco termo elastic properties of a polymer interlayer by dynamic tests Laura Andreozzi 1, Silvia Briccoli Bati 2, Mario Fagone 2 Giovanna Ranocchiai 2 Fabio Zulli 1 1 Department
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 3 VISCOELASTICITY. k a. N t
MATERIAL MECHANICS, SE2126 COMPUTER LAB 3 VISCOELASTICITY N t i Gt () G0 1 i ( 1 e τ = α ) i= 1 k a k b τ PART A RELAXING PLASTIC PAPERCLIP Consider an ordinary paperclip made of plastic, as they more
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationAspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites
Aspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites J.A.Nairn Wood Science and Engineering, Oregon State University, Corvallis, OR 97330, USA Abstract A fiber s efficiency in a
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationA simple planestrain solution for functionally graded multilayered isotropic cylinders
Structural Engineering and Mechanics, Vol. 24, o. 6 (2006) 000000 1 A simple planestrain solution for functionally graded multilayered isotropic cylinders E. Pan Department of Civil Engineering, The
More informationarxiv: v1 [condmat.soft] 26 Dec 2015
Surface tension and the MoriTanaka theory of nondilute soft composite solids arxiv:52.08089v [condmat.soft] 26 Dec 205 Francesco Mancarella, Robert W. Style, 2, 2, and John S. Wettlaufer Nordic Institute
More informationStressinduced transverse isotropy in rocks
Stanford Exploration Project, Report 80, May 15, 2001, pages 1 318 Stressinduced transverse isotropy in rocks Lawrence M. Schwartz, 1 William F. Murphy, III, 1 and James G. Berryman 1 ABSTRACT The application
More informationUniversity Graz / Austria Institut für Chemie Volker Ribitsch
University Graz / Austria Institut für Chemie Volker Ribitsch 1 Rheology Oscillatory experiments Dynamic experiments Deformation of materials under nonsteady conditions in the linear viscoelastic range
More informationLectures on. Constitutive Modelling of Arteries. Ray Ogden
Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics
More informationFrequency Response of Composite Laminates at Various Boundary Conditions
International Journal of Engineering Science Invention (IJESI) ISSN (Online): 2319 6734, ISSN (Print): 2319 6726 www.ijesi.org ǁ PP.1115 Frequency Response of Composite Laminates at Various Boundary Conditions
More informationReduced warp in torsion of reticulated foam due to Cosserat elasticity: experiment
Reduced warp in torsion of reticulated foam due to Cosserat elasticity: experiment Roderic S. Lakes May 25, 2016 Department of Engineering Physics, Department of Materials Science University of Wisconsin,
More informationU.S. South America Workshop. Mechanics and Advanced Materials Research and Education. Rio de Janeiro, Brazil. August 2 6, Steven L.
Computational Modeling of Composite and Functionally Graded Materials U.S. South America Workshop Mechanics and Advanced Materials Research and Education Rio de Janeiro, Brazil August 2 6, 2002 Steven
More informationNANOINDENTATION STUDIES OF PAPER
Progress in Paper Physics Seminar 2008  June 25, Otaniemi Finland NANOINDENTATION STUDIES OF PAPER B. F. West 1, B. T. Hotle 2, J. E. Jakes 3,4, J. M. Considine 3, R. E. Rowlands 1 and K. T. Turner 1,4
More informationAnalysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements
Acta Mech. Sin. (2016) 32(2):295 300 DOI 10.1007/s1040901505342 RESEARCH PAPER Analysis of the geometrical dependence of auxetic behavior in reentrant structures by finite elements V. H. Carneiro 1
More informationFigure 1. Dimension of PSA in face paper laminate
EVALUATION OF DYNAMIC MECHANICAL PROPERTIES OF PRESSURE SENSITIVE ADHESIVE IN PAPER LANIMATES FOR POSTAGE STAMP APPLICATION: METHOD DEVELOPMENT AND ADHESIVE CHARACTERIZATION Hailing Yang, Graduate Student,
More informationEXPERIMENTAL STUDY ON YOUNG S MODULUS E OF A POLYMER COMPOSITE REINFORCED BY NANO TITANIUM DIOXIDE PARTICLES
Vietnam Journal of Mechanics, VAST, Vol. 34, No. (202), pp. 9 25 EXPERIMENTAL STUDY ON YOUNG S MODULUS E OF A POLYMER COMPOSITE REINFORCED BY NANO TITANIUM DIOXIDE PARTICLES Nguyen Dinh Duc, Dinh Khac
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationTHE BENDING STIFFNESSES OF CORRUGATED BOARD
AMDVol. 145/MDVol. 36, Mechanics of Cellulosic Materials ASME 1992 THE BENDING STIFFNESSES OF CORRUGATED BOARD S. Luo and J. C. Suhling Department of Mechanical Engineering Auburn University Auburn,
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationSEISMIC BASE ISOLATION
SEISMIC BASE ISOLATION DESIGN OF BASE ISOLATION SYSTEMS IN BUILDINGS FILIPE RIBEIRO DE FIGUEIREDO SUMMARY The current paper aims to present the results of a study for the comparison of different base isolation
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationModeling Contact between Rigid Sphere and Elastic Layer Bonded to Rigid Substrate
IEEE TRANSACTIONS ON COMPONENTS AND PACKAGING TECHNOLOGIES, VOL. 24, NO. 2, JUNE 2001 207 Modeling Contact between Rigid Sphere and Elastic Layer Bonded to Rigid Substrate Mirko Stevanović, M. Michael
More informationComputer Methods in Applied Mechanics and Engineering, 66, (1988).
1 FINITE ELEMENT ANALYSIS OF STRESS CONCENTRATION AROUND A BLUNT CRACK IN A COSSERAT ELASTIC SOLID S. Nakamura and R.S. Lakes adapted from Computer Methods in Applied Mechanics and Engineering, 66, 257266
More informationPolymer engineering syllabus (BSc)
Polymer engineering syllabus (BSc) First semester Math 1 Physics 1 Physics 1 lab General chemistry General chemistry lab workshop Second semester Math 2 Physics 2 Organic chemistry 1 Organic chemistry
More informationTesting and Analysis
Testing and Analysis Testing Elastomers for Hyperelastic Material Models in Finite Element Analysis 2.6 2.4 2.2 2.0 1.8 1.6 1.4 Biaxial Extension Simple Tension Figure 1, A Typical Final Data Set for Input
More information6.730 Physics for Solid State Applications
6.730 Physics for Solid State Applications Lecture 5: Specific Heat of Lattice Waves Outline Review Lecture 4 3D Elastic Continuum 3D Lattice Waves Lattice Density of Modes Specific Heat of Lattice Specific
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationA discrete element analysis of elastic properties of granular materials
Granular Matter (213) 15:139 147 DOI 1.17/s13513393 ORIGINAL PAPER A discrete element analysis of elastic properties of granular materials X. Q. Gu J. Yang Received: 13 October 212 / Accepted: 1 January
More informationA New Ultrasonic Immersion Technique to Retrieve Anisotropic Stiffness Matrix for Dispersion Curves Algorithms
A New Ultrasonic Immersion Technique to Retrieve Anisotropic Stiffness Matrix for Dispersion Curves Algorithms DARUN BARAZANCHY 1, WILLIAM ROTH 2 and VICTOR GIURGIUTIU 3 ABSTRACT Dispersion curve algorithms
More informationA differential scheme for elastic properties of rocks with dry or saturated cracks
Geophys. J. Int. (2002, 597 6 A differential scheme for elastic properties of rocks with dry or saturated cracks James G. Berryman, Steven R. Pride 2 and Herbert F. Wang 3 University of California, Lawrence
More informationBME 207 Introduction to Biomechanics Spring 2017
April 7, 2017 UNIVERSITY OF RHODE ISAND Department of Electrical, Computer and Biomedical Engineering BE 207 Introduction to Biomechanics Spring 2017 Homework 7 Problem 14.3 in the textbook. In addition
More informationChapter 6: Mechanical Properties of Metals. Dr. Feras Fraige
Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness
More informationDynamic Mechanical Analysis of Solid Polymers and Polymer Melts
Polymer Physics 2015 Matilda Larsson Dynamic Mechanical Analysis of Solid Polymers and Polymer Melts Polymer & Materials Chemistry Introduction Two common instruments for dynamic mechanical thermal analysis
More informationGraduate School of Engineering, Kyoto University, Kyoto daigakukatsura, Nishikyoku, Kyoto, Japan.
On relationship between contact surface rigidity and harmonic generation behavior in composite materials with mechanical nonlinearity at fibermatrix interface (Singapore November 2017) N. Matsuda, K.
More informationA differential scheme for elastic properties of rocks with dry or saturated cracks
Stanford Exploration Project, Report 08, April 29, 200, pages?? A differential scheme for elastic properties of rocks with dry or saturated cracks James G. Berryman, Steven R. Pride, 2 and Herbert F. Wang
More informationVariational bounds for anisotropic elastic multiphase composites with different shapes of inclusions
Arch Appl Mech DOI 1.17/s41982461 ORIGINAL R. RodríguezRamos R. GuinovartDíaz J. BravoCastillero F. J. Sabina H. Berger S. Kari U. Gabbert Variational bounds for anisotropic elastic multiphase composites
More informationOPTIMISING THE MECHANICAL CHARACTERISATION OF A RESILIENT INTERLAYER FOR THE USE IN TIMBER CON STRUCTION
OPTIMISING THE MECHANICAL CHARACTERISATION OF A RESILIENT INTERLAYER FOR THE USE IN TIMBER CON STRUCTION Luca Barbaresi, Federica Morandi, Juri Belcari, Andrea Zucchelli and Alice Speranza University
More informationMechanical Behavior of Fullerene Reinforced Fiber Composites with Interface Defects through Homogenization Approach and Finite Element Method
, pp.6782 http://dx.doi.org/1.14257/ijast.215.78.6 Mechanical Behavior of Fullerene Reinforced Fiber Composites with Interface Defects through Homogenization Approach and Finite Element Method P. Prasanthi
More informationEntanglements. M < M e. M > M e. Rouse. Zeroshear viscosity vs. M (note change of slope) Edwards degennes Doi. Berry + Fox, slope 3.4.
Entanglements Zeroshear viscosity vs. M (note change of slope) M < M e Rouse slope 3.4 M > M e Edwards degennes Doi slope 1 Berry + Fox, 1968 Question: Which factors affect the Me: T, P, M, flexibility,
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationThe concept of Representative Volume for elastic, hardening and softening materials
The concept of Representative Volume for elastic, hardening and softening materials Inna M. Gitman Harm Askes Lambertus J. Sluys Oriol Lloberas Valls i.gitman@citg.tudelft.nl Abstract The concept of the
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationMechanical Metamaterials. Graeme W. Milton University of Utah
Mechanical Metamaterials Graeme W. Milton University of Utah Walser 1999: Macroscopic composites having a manmade, threedimensional, periodic cellular architecture designed to produce an optimized combination,
More informationMethane hydrate rock physics models for the Blake Outer Ridge
Stanford Exploration Project, Report 80, May 15, 2001, pages 1 307 Methane hydrate rock physics models for the Blake Outer Ridge Christine Ecker 1 ABSTRACT Seismic analyses of methane hydrate data from
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationSize Effect of Clay Filler Particles on Mechanical Properties of Pultruded Polymer Composites Under Shear Loading
Minnesota State University, Mankato Cornerstone: A Collection of Scholarly and Creative Works for Minnesota State University, Mankato All Theses, Dissertations, and Other Capstone Projects Theses, Dissertations,
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationClass XI Physics. Ch. 9: Mechanical Properties of solids. NCERT Solutions
Downloaded from Class XI Physics Ch. 9: Mechanical Properties of solids NCERT Solutions Page 242 Question 9.1: A steel wire of length 4.7 m and crosssectional area 3.0 10 5 m 2 stretches by the same amount
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationLinear Cosserat elasticity, conformal curvature and bounded stiffness
1 Linear Cosserat elasticity, conformal curvature and bounded stiffness Patrizio Neff, Jena Jeong Chair of Nonlinear Analysis & Modelling, Uni Dui.Essen Ecole Speciale des Travaux Publics, Cachan, Paris
More informationElastic Properties of Polycrystalline Solid Helium
JLowTempPhys(2010)160:5 11 DOI 10.1007/s1090901001738 Elastic Properties of Polycrystalline Solid Helium Humphrey J. Maris Sebastien Balibar Received: 29 March 2010 / Accepted: 16 April 2010 / Published
More informationA CRITERION OF TENSILE FAILURE FOR HYPERELASTIC MATERIALS AND ITS APPLICATION TO VISCOELASTICVISCOPLASTIC MATERIALS
MTS ADHESIVES PROGRAMME 19961999 PERFORMANCE OF ADHESIVE JOINTS Project: PAJ1; Failure Criteria and their Application to ViscoElastic/ViscoPlastic Materials Report 2 A CRITERION OF TENSILE FAILURE FOR
More informationControlling elastic wave with isotropic transformation materials
Controlling elastic wave with isotropic transformation materials Zheng Chang, Jin Hu, a, Gengkai Hu, b, Ran Tao and Yue Wang School of Aerospace Engineering, Beijing Institute of Technology, 0008,Beijing,
More informationEffective Medium Theories Effective Medium Models
Effective Medium Models 3 Bounding Methods for Estimating Effective Elastic Moduli For many reasons we would like to be able to model or estimate the effective elastic moduli of rocks in terms of the properties
More informationEvaluation of damping and elastic properties of composites and composite structures by the resonance technique
JOURNAL OF MATERIALS SCIENCE 35 (2000)3785 3792 Evaluation of damping and elastic properties of composites and composite structures by the resonance technique C. Y. WEI, S. N. KUKUREKA The University of
More informationRheology, Adhesion, and Debonding of Lightly Crosslinked Polymer Gels
Rheology, Adhesion, and Debonding of Lightly Crosslinked Polymer Gels Nicholas B. Wyatt, and Anne M. Grillet 2 Materials Science and Engineering Division 2 Engineering Sciences Division Sandia National
More informationPeriod #1 : CIVIL MATERIALS COURSE OVERVIEW
Period #1 : CIVIL MATERIALS COURSE OVERVIEW A. Materials Systems to be Addressed Metals and Alloys (steel and aluminum) Portland Cement Concrete Asphalt Cement Concrete Fiber Reinforced Composites Masonry
More informationThe Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
11th European Conference on NonDestructive Testing (ECNDT 214), October 61, 214, Prague, Czech Republic The Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
More informationThe Large Amplitude Oscillatory Strain Response of Aqueous Foam: Strain Localization and Full Stress Fourier Spectrum
The Large Amplitude Oscillatory Strain Response of Aqueous Foam: Strain Localization and Full Stress Fourier Spectrum By F. Rouyer, S. CohenAddad, R. Höhler, P. Sollich, and S.M. Fielding The European
More informationMicrostructure design of a two phase composite using twopoint correlation functions
Brigham Young University BYU ScholarsArchive All Faculty Publications 20040101 Microstructure design of a two phase composite using twopoint correlation functions Brent L. Adams b_l_adams@byu.edu H.
More informationDevelopment of a Rubber for a Tuned Mass Damper for Rail Vibration
Development of a Rubber for a Tuned Mass Damper for Rail Vibration A H Muhr For RIEG Discussion Meeting on Vibration Control with Elastomer Products DTR VMS, Trowbridge, 6 th June 2014 Based on PhD thesis
More informationA MultiPhysics Study of the Wave Propagation Problem in Open Cell Polyurethane Foams
A MultiPhysics Study of the Wave Propagation Problem in Open Cell Polyurethane Foams M. Brennan 1, M. Dossi 1, M. Moesen 1 1. Huntsman Polyurethanes, Everslaan 45, 3078 Everberg, Belgium. Abstract Flexible
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationComputational Modelling of Vibrations Transmission Loss of Auxetic Lattice Structure
Vibrations in Physical Systems Vol. 27 (2016) Abstract Computational Modelling of Vibrations Transmission Loss of Auxetic Lattice Structure Eligiusz IDCZAK Institute of Applied Mechanics, Poznan University
More information